ASSESSMENT OF WHISKER GROWTHFROM TIN COATED WIRE AND CABLE Tom Lesniewski Northrop Grumman CorporationSan Diego, CA
Objective “What is the risk for whisker growth on tin-coated wire?”
Topics • Standards • Historical data • Analysis--variables • Wire gauge • Age • Type of pure tin coating/grain size • Results • SEM inspection • Cross section
Wire & Cable Standards • Pure tin is a common finish for copper wire and cable • MIL-DTL-17 coaxial cable • AA-59551 (ss QQ-W-343) uninsulated “bus” wire • NEMA-WC27500 (ss MIL-DTL-27500) cable • SAE-AS22759 (ss MIL-W-22759) and MIL-DTL-16878 insulated wire • Wire call-outs trace back to ASTM B33 • No restrictions or guidance on pure tin
Wire & Cable Standards • ASTM B33 does not specify a tin coating thickness “It is necessary that the coating of tin on the wire be continuous.” • Tin coating consists of 2 parts • Pure tin coating at surface • Intermetallic compounds between tin & copper
Wire & Cable Standards • Most common type of uninsulated wire: QQ-W-343 (superseded by AA-59551) • Two types: • Type S wire –single stranded, uninsulated • Tin coating is 40 uin (1 um) thick minimum. • Thick enough to protect copper & prevent corrosion but limited shelf life • 1 um coating will not pass solderability test after steam aging due to oxidation of IMCs • Type H wire --“hookup wire” • Additional solderability requirement (steam age) • Thicker tin coating, typically 300 uin (7.7 um) or more
Literature / Historical Data • Sparse citations of whisker growth on tin plated wire • Bell Labs studies in the 1950s and 60s • On tin coated wire, “short whiskers, relatively few in number, were found” • NASA Goddard tin whisker website: whiskers on diode wire leads, • Wire manufacturers: handful of customer reports of whiskers on tin coated wire over past 20 years, all on type H wire. • Several references suggest that there is little to no risk for substantial whisker growth on tin coated wire and cable. • No whiskers found on tin-coated wire on Titan missile harnesses • MIL-STD-1547 (“Electronic Parts, Materials and Processes for Space and Launch Vehicles rev B”) includes an exemption for tin plated drawn wire products, such as cables, shielding and ground straps.
Analysis • 20 samples of tin-coated wire, cable & braid • Manufactured between 1965 and 2008 • 10 different suppliers • Type S and H • Two samples temperature cycled for 1000 cycles between -40 and 100°C • Analysis • Microscope inspection • Energy Dispersive Xray (EDX)--material composition • Scanning Electron Microscopy (SEM)--size and density of whiskers, grain size • Cross section--intermetallic compound and tin layer thickness • One electroplated mechanical part included for comparison
EDX/SEM Inspection • EDX confirmed pure tin coating over copper wire
EDX/SEM Inspection • None of the 20 wire and braid samples showed whiskers
EDX/SEM Inspection • Braid samples showed some flat strands, believed to be “burrs” incurred from manufacturing process • Electroplated terminal lug showed profuse whiskering Tin plated copper terminal lug Tin plated copper braid
Cross Sections Sample 2 7 year old bus wire IMC consumes 30 to 100% of tin layer
Cross Sections ← Sample 5 23 year old braid (type S wire) IMC consumes 100% of tin layer Sample 11 → 43 year old type H wire IMC consumes 20% of tin layer
IMC Thickness • General trend of increasing IMC thickness with age. • Outliers (samples 17 and 23) have much thicker tin layer
IMC Thickness • Type S coatings are consumed by IMC in first years • Type H coatings retain 50-75% of nascent pure tin
Wire Manufacturing Processes • Two processes used to coat bare copper wire with tin: electroplating (aka electrodeposit) and hot dipping. • Plating = electrochemical process • Hot dipping = physical process • Regardless of the coating process, the bare copper wire is processed the same • Copper rods or bars heated and drawn through a series of dies to reduce diameter • Drawing is similar to extrusion except that the wire is pulled through the die rather than pushed
Copper drawn & rolled Copper heat treat (500 to 850°C) Tin electroplate (35°C) Wire draw & anneal (200°C) Quench Spool Copper drawn & rolled Copper heat treat (500 to 850°C) Tin electroplate (35°C) Spool Copper heat treat (500 to 850°C) Hot tin dip (250° C) Wipe excess tin Spool Copper drawn & rolled Wire Manufacturing Processes Type S electroplated tin coated copper wire Type H electroplated tin coated copper wire Type S hot dipped tin coated copper wire
Significant differences between hot dipping and electroplating: • Hot dipping takes place at much higher temperature, therefore resulting in thicker initial IMC. • Hot dipped wire is handled in the molten state to remove excess tin; processes may be variable. • Hot dipped wire produces smaller, less distinct grains • Type S electroplated wire is drawn through a die after plating
Grain structure & size- sample 23 (plated lug) Electroplated wire shows larger, more distinct grains with sharp ridges. Grain size is 3.9 ± 1.8 μm
Grain Structure & Growth-Sample 4 (hot dipped braid) Hot dipped wire shows relatively smooth, shows signs of reflow with less structured grains. Grain size 1.3 ± 0.6 μm
Conclusions • Three factors work to suppress whisker growth on wires • Post-plating drawing steps cold work the wire • Annealing relieves stresses in the plating • Larger IMC layer in hot dipped wire results in less pure tin material available for whisker growth. • Thus type S wires (hot dipped or electroplated) would tend to be at lower risk for whisker growth than wires with thicker plating (type H). • According to QQ-W-343 & AA-59551, Type H wire is preferred as hookup wire on electrical assemblies because of its solderability • In terms of whisker mitigation, however, type S wire is preferred to type H.
Conclusions • No tin whiskers were observed on any samples; 20 samples from 10 suppliers, aged between 1 and 44 years. • No correlation between whisker growth and age of sample, intermetallic compound thickness, supplier or coating process (hot dipped vs. electroplated). • Significant differences between tin plated wire (no whiskers) and tin plated component terminations (whiskers) include geometry, thickness of tin layer, and post plating annealing and cold working processes. None of these factors alone appear to be completely successful in suppressing whiskers; rather it is likely a combination of factors. • Literature contains four reports of whisker growth on tin plated copper wire or wire leads (refs 8,9,10,11) • Interviews with wire manufacturers revealed isolated reports of tin whiskers on wire over the past 20 years. • Several data-based references state that there is little to no risk for substantial whisker growth on tin-plated wire and cable.